Strength and Water Absorption of Sustainable Concrete Produced with Recycled Basaltic Concrete Aggregates and Powder

: In this study, the recycled concrete aggregates and powder (RCA and RCP) prepared from basaltic concrete waste were used to replace the natural aggregate (NA) and cement, respectively. The NA (coarse and ﬁne) was replaced by the recycled aggregates with ﬁve percentages (0%, 20%, 40%, 60% and 80%). Consequently, the cement was replaced by the RCP with four percentages (0%, 5%, 10% and 20%). Cubes with 100 mm edge length were prepared for all tests. The compressive and tensile strengths ( f cu and f tu ) and water absorption (WA) were investigated for all mixes at different ages. Partial substitution of NA with recycled aggregate reduced the compressive strength with different percentages depending on the type and source of recycled aggregate. After 28 days, the maximum reduction in f cu value was 9.8% and 9.4% for mixtures with coarse RCA and ﬁne RCA (FRCA), respectively. After 56 days, the mixes with 40% FRCA reached almost the same f cu value as the control mix (M0, 99.5%). Consequently, the compressive strengths of the mixes with 10% RCA at 28 and 56 days were 99.3 and 95.2%, respectively, compared to those of M0. The mixes integrated FRCA and RCP showed higher tensile strengths than the M0 at 56 d with a very small reduction at 28 d (max = 3.4%). Moreover, the f cu and f tu values increased for the late test ages, while the WA decreased.


Introduction
Nowadays, a lot of attention is paid to the sustainable disposal of construction waste and its management, as it decreases the cost of disposal and reduces the environmental impact (EI) [1]. The construction industry has caused high environmental impacts worldwide as it demands excessive extraction of raw materials. Sand and gravel are the highest materials that are used on Earth next to water in contrast, and their natural regeneration rates are significantly lower than their usages as was specified by the United Nations Environment Programme. Natural aggregates of about 45 billion tons were extracted in 2017 and they are estimated to rise to 66 billion tons in 2025. Moreover, about 40 billion tons/year from aggregates were consumed in the cement product industries worldwide [2][3][4]. Furthermore, the European Statistical Office reported that about 923 billion tons/year of industrial wastes are produced from the construction works. The wastes generated from the construction The use of concrete waste as a recycled aggregate is popular to produce new co In contrast, the use of concrete waste powder as a cement substitute is still limite hough the basaltic concrete waste has a pozzolanic effect, the use of this waste as a tute for aggregate and cement is still limited. In this study, the use of basaltic c waste as a substitute for natural aggregates with low and high content was inves In addition, the use of basaltic concrete powder, that had pozzolanic activity, to cement and produce sustainable/green concrete was also investigated.  Table 1.

Recycled Concrete Aggregates
The recycled basaltic concrete is taken from old concrete cubes and cylinders that were tested in the lab five to six years ago for previous research projects and kept outside the lab as wastes. The old cubes and cylinders were manually crushed then put in a crushing machine to obtain RCA, FRCA and powder. The concrete strength of the old concrete ranged from 33 MPa to 39 MPa. The CRCA and FRCA obtained from the basalt concrete are shown in Figure 1c,d, respectively. The standard sieves were used to separate the basaltic concrete wastes (BCWs) into CRCA, FRCA and RCP. The CRCA remaining on sieve No. 4 (sieve opening = 4.75 mm) was used as a replacement for the coarse NA. The MNS of the CRCA used in this experimental program was adjusted to correspond to 12.5 mm. The selected MNS (12.5 mm) was adopted to minimize the negative effects of the FRCA compared to other larger sizes (19 and 25 mm) on the durability and strength of the concrete [64]. Consequently, the FRCA that passed the No. 4 sieve and remained on the No. 100 sieve (sieve opening = 150 microns) were used to replace the fine NA (sand). The fineness modulus of the FRCA was also equal to 3.2. The particle size distribution curves of the CRCA and FRCA were adjusted to comply with the limits of ASTM C33 [63] ( Figure  2b). The physical properties of CRCA and FRCA are listed in Table 1.

Recycled Concrete Powder
The RCP passed from sieve No. 100 during sieve analysis of BCWs is shown in Figure  1e. The RCP was analyzed by scanning electron microscope (SEM and EDS) to find its chemical components. The obtained chemical components from EDS analysis are listed in Table 2, while the photos of EDS and SEM are shown in Figure 3a

Recycled Concrete Aggregates
The recycled basaltic concrete is taken from old concrete cubes and cylinders that were tested in the lab five to six years ago for previous research projects and kept outside the lab as wastes. The old cubes and cylinders were manually crushed then put in a crushing machine to obtain RCA, FRCA and powder. The concrete strength of the old concrete ranged from 33 MPa to 39 MPa. The CRCA and FRCA obtained from the basalt concrete are shown in Figure 1c,d, respectively. The standard sieves were used to separate the basaltic concrete wastes (BCWs) into CRCA, FRCA and RCP. The CRCA remaining on sieve No. 4 (sieve opening = 4.75 mm) was used as a replacement for the coarse NA. The MNS of the CRCA used in this experimental program was adjusted to correspond to 12.5 mm. The selected MNS (12.5 mm) was adopted to minimize the negative effects of the FRCA compared to other larger sizes (19 and 25 mm) on the durability and strength of the concrete [64]. Consequently, the FRCA that passed the No. 4 sieve and remained on the No. 100 sieve (sieve opening = 150 microns) were used to replace the fine NA (sand). The fineness modulus of the FRCA was also equal to 3.2. The particle size distribution curves of the CRCA and FRCA were adjusted to comply with the limits of ASTM C33 [63] ( Figure 2b). The physical properties of CRCA and FRCA are listed in Table 1.

Recycled Concrete Powder
The RCP passed from sieve No. 100 during sieve analysis of BCWs is shown in Figure 1e. The RCP was analyzed by scanning electron microscope (SEM and EDS) to find its chemical components. The obtained chemical components from EDS analysis are listed in Table 2, while the photos of EDS and SEM are shown in Figure 3a,b, respectively.

Cement
The OPC produced locally in one of the Cement Factories in KSA was used for all concrete mixes. The chemical composition of this cement as provided by the supplier is also given in Table 2.

Validation of the Material Chemical Composition as Natural Pozzolana
The chemical properties of the basaltic concrete powder are shown in Table 1. The chemical composition of RCP is underlain by silica (SiO2). ASTM C618 recommends a sum of SiO2, Fe2O3, and Al2O3 greater than 70% for the chemical composition requirements of natural pozzolana. According to Table 2, the sum of SiO2, Fe2O3, and Al2O3 for RCP (87.68%) meets the ASTM C618 requirements for natural pozzolana. Therefore, the utilization of RCA as fine and coarse aggregate and RCP as a waste powder in the hydration process can help to produce sustainable concrete based on basalt waste.

Mix Proportions and Mixing Procedure
In this work, a control mix (M0) was designated according to the ACI specification [65] to obtain 35 MPa cylindrical concrete strength at 28 days. The M0 mix was designated to keep a slump of 50-80 mm and mechanical compaction was used. The CRCA and FRCA gradings were adopted to be like that for NA. The W/C ratio for M0 was adopted to be 0.5. For mixes with recycled aggregate, the recycled aggregate was used to partially replaced the natural aggregate by weight. All the aspects remained unchanged to study the effects of replacing this recycled aggregate with their different physical properties on the concrete mechanical properties and water absorption. Most previous studies neglected the humidity and water absorption when designing the concrete mixes with or without recycled materials [18,[51][52][53]. The mix M0 was prepared, and its slump was obtained. The slump of M0 mix achieved the required slump with neglecting the humidity and water content of the aggregates. For mixes incorporating RCA, the additional water required for each mix to keep the same consistency of M0 mix was calculated and added during mixing (Figure 4a). The mix (M0) consisted of natural sand, natural basalt and OPC with weight

Cement
The OPC produced locally in one of the Cement Factories in KSA was used for all concrete mixes. The chemical composition of this cement as provided by the supplier is also given in Table 2.

Validation of the Material Chemical Composition as Natural Pozzolana
The chemical properties of the basaltic concrete powder are shown in Table 1. The chemical composition of RCP is underlain by silica (SiO 2 ). ASTM C618 recommends a sum of SiO 2 , Fe 2 O 3 , and Al 2 O 3 greater than 70% for the chemical composition requirements of natural pozzolana. According to Table 2, the sum of SiO 2 , Fe 2 O 3 , and Al 2 O 3 for RCP (87.68%) meets the ASTM C618 requirements for natural pozzolana. Therefore, the utilization of RCA as fine and coarse aggregate and RCP as a waste powder in the hydration process can help to produce sustainable concrete based on basalt waste.

Mix Proportions and Mixing Procedure
In this work, a control mix (M0) was designated according to the ACI specification [65] to obtain 35 MPa cylindrical concrete strength at 28 days. The M0 mix was designated to keep a slump of 50-80 mm and mechanical compaction was used. The CRCA and FRCA gradings were adopted to be like that for NA. The W/C ratio for M0 was adopted to be 0.5. For mixes with recycled aggregate, the recycled aggregate was used to partially replaced the natural aggregate by weight. All the aspects remained unchanged to study the effects of replacing this recycled aggregate with their different physical properties on the concrete mechanical properties and water absorption. Most previous studies neglected the humidity and water absorption when designing the concrete mixes with or without recycled materials [18,[51][52][53]. The mix M0 was prepared, and its slump was obtained. The slump of M0 mix achieved the required slump with neglecting the humidity and water content of the aggregates. For mixes incorporating RCA, the additional water required for each mix to keep the same consistency of M0 mix was calculated and added during mixing (Figure 4a).
The mix (M0) consisted of natural sand, natural basalt and OPC with weight percentages of 643, 1016 and 400 kg/m 3 respectively ( Table 3). The effect of the CRCA and FRCA on the W/C is also shown in Figure 4b. In order to produce sustainable concrete, eleven mixes (M1 to M11) were prepared in which the natural concrete constituents (aggregates and cement) were replaced by the recycled waste materials in different proportions. For the mixes M1-M4, the CRCA was used to replace the coarse NA with five percentages (0%, 20%, 40%, 60% and 80%, respectively). For mixtures M5-M8, natural sand was replaced with FRCA at five percentages (0%, 20%, 40%, 60%, and 80%, respectively). In addition, for mixes M9-M11, OPC was replaced with RCP at four percentages (0%, 5%, 10%, and 20%, respectively). Full details of the mix proportions for all mixes are summarized in Table 3. The aggregates and cement were dry mixed in the concrete mixer for 1 min. The RCP (if any) was then added and dry mixed for another 1 min. Then, the water was added gradually, and mixing was completed for another 2 min. The concrete mixtures were poured into 100 × 100 × 100 mm 3 cubes. The cubes were de-moulded after 24 h and cured in a water tank until the test age (7, 28, and 56 days).  (Table 3). The effect of the CRCA and FRCA on the W/C is also shown in Figure 4b. In order to produce sustainable concrete, eleven mixes (M1 to M11) were prepared in which the natural concrete constituents (aggregates and cement) were replaced by the recycled waste materials in different proportions. For the mixes M1-M4, the CRCA was used to replace the coarse NA with five percentages (0%, 20%, 40%, 60% and 80%, respectively). For mixtures M5-M8, natural sand was replaced with FRCA at five percentages (0%, 20%, 40%, 60%, and 80%, respectively). In addition, for mixes M9-M11, OPC was replaced with RCP at four percentages (0%, 5%, 10%, and 20%, respectively). Full details of the mix proportions for all mixes are summarized in Table 3. The aggregates and cement were dry mixed in the concrete mixer for 1 min. The RCP (if any) was then added and dry mixed for another 1 min. Then, the water was added gradually, and mixing was completed for another 2 min. The concrete mixtures were poured into 100 × 100 × 100 mm 3 cubes. The cubes were de-moulded after 24 h and cured in a water tank until the test age (7, 28, and 56 days).

Test Method
To evaluate the compressive strengths of all mixes, the 100-mm cube specimens were compression tested at 7, 28, and 56 days according to BS EN 12390-3 [66]. At each age, the results of three tested cubes were averaged to obtain the compressive strength (f cu ). The concrete tensile strengths (f tu ) at 28 and 56 d were also obtained from the diagonal splitting test for the cubes with 100 mm edge length, as shown in Figure 5 and Equation (1) [67].
where b and d are the width and diagonal length of the cube, and P is the maximum compressive load. In this study, the value of β is equal to 0.15. At each age, the results of three tested cubes were averaged to obtain the tensile strength (f tu ). The compression testing machine with a maximum capacity of 2000 tons was used to test the cubes in compression and in tension at a loading rate of 4 and 3 kN/s, respectively. Water absorption (WA) is one of the well-known concrete durability factors [47,68,69]. Moreover, WA of concrete was considered as a measure for resistance against carbonation and chloride migration [70].
WA was obtained according to ASTM C642 [71] to compare the durability of the mixes after 28 and 56 days. First, the concrete specimens (3 cubes at each age) were dried at a temperature (T) of 100-110 • C for more than 24 h to find the oven-dried mass (A) in grams. Subsequently, the samples were engrossed in water at T ≈ 21 • C for more than 48 h, then the surface-dried samples were weighed in grams (B), and then WA was calculated according to Equation (2).

Test Method
To evaluate the compressive strengths of all mixes, the 100-mm cube specimens were compression tested at 7, 28, and 56 days according to BS EN 12390-3 [66]. At each age, the results of three tested cubes were averaged to obtain the compressive strength (fcu). The concrete tensile strengths (ftu) at 28 and 56 d were also obtained from the diagonal splitting test for the cubes with 100 mm edge length, as shown in Figure 5 and Equation (1) [67].
where b and d are the width and diagonal length of the cube, and P is the maximum compressive load. In this study, the value of β is equal to 0.15. At each age, the results of three tested cubes were averaged to obtain the tensile strength (ftu). The compression testing machine with a maximum capacity of 2000 tons was used to test the cubes in compression and in tension at a loading rate of 4 and 3 kN/s, respectively. Water absorption (WA) is one of the well-known concrete durability factors [47,68,69]. Moreover, WA of concrete was considered as a measure for resistance against carbonation and chloride migration [70]. WA was obtained according to ASTM C642 [71] to compare the durability of the mixes after 28 and 56 days. First, the concrete specimens (3 cubes at each age) were dried at a temperature (T) of 100-110 °C for more than 24 h to find the oven-dried mass (A) in grams. Subsequently, the samples were engrossed in water at T ≈ 21 °C for more than 48 h, then the surface-dried samples were weighed in grams (B), and then WA was calculated according to Equation (2).

Concrete Compressive Strength
The cubic concrete strengths (fcu) at 7, 28, and 56 days of age (fcu,7, fcu,28, and fcu,56, respectively) are shown in Table 4. The reduction values of concrete strength at 7, 28, and 56 days (µ7, µ28, and µ56) due to partial replacement of natural basalt, sand and cement by the recycled waste are also presented in Table 4. The percentage increase in fcu,28 compared to fcu,7 (µ28/7) and fcu,56 compared to fcu,28 (µ56/28) for all the tested mixes are also presented in Table 4. The effect of recycled waste on compressive strengths is discussed in the following sections. The percentage compressive strength decreases at each curing time (µcu,date%) is calculated using Equation (3).

Concrete Compressive Strength
The cubic concrete strengths (f cu ) at 7, 28, and 56 days of age (f cu,7 , f cu,28 , and f cu,56 , respectively) are shown in Table 4. The reduction values of concrete strength at 7, 28, and 56 days (µ 7 , µ 28 , and µ 56 ) due to partial replacement of natural basalt, sand and cement by the recycled waste are also presented in Table 4. The percentage increase in f cu,28 compared to f cu,7 (µ 28/7 ) and f cu,56 compared to f cu,28 (µ 56/28 ) for all the tested mixes are also presented in Table 4. The effect of recycled waste on compressive strengths is discussed in the following sections. The percentage compressive strength decreases at each curing time (µ cu,date %) is calculated using Equation (3).
where f cu , date (R) and f cu,date (N) are the compressive strengths of the mixtures that integrate waste and the control mixture, respectively.  (Figure 6a). Comparing the strengths obtained at 7 and 56 days with those obtained at 28 days, they showed higher rates of strength increase when Tc was increased from 7 to 28 days than when Tc was increased from 28 to 56 days. This may be due to the higher cement hydration rates during the first 28 days compared to the late days. they showed higher rates of strength increase when Tc was increased from 7 to 28 days than when Tc was increased from 28 to 56 days. This may be due to the higher cement hydration rates during the first 28 days compared to the late days. The increase in strengths with increasing curing age was also related to CRCA%. When Tc increased from 7 to 28 days, the strength increased by 27.8%, 39.6%, 35.2, 32.5 and 33.4% for M0 to M4, respectively, illustrating the influence of CRCA% on early cement hydration. Consequently, the strength increased with increasing Tc from 28 to 56 d by 14.7%, 13.9%, 14.3%, 12.8% and 7.9% for M0 to M4, respectively. The low increase in strength at 56 days for the mixes integrating CRCA% than that of M0 ensured the effect of crushed concrete and its voids on the absorption of water required to complete cement hydration. The replacement of coarse NA with CRCA generally reduced the concrete strength. The CRCA are made of recycled basalt, and crushed concrete, which had a high void ratio compared to NA, and can affect concrete strength and cement hydration in addition to the powder. Strength reduction was strongly influenced by CRCA% and curing age. After 7 days, the strength reduction (µ7%) is 17.3%, 13.9%, 10.8%, and 16.7% for mixtures with CRCA content of 20%, 40%, 60%, and 80%, respectively (mean (µ) = 14.8% and standard deviation (σµ) = ±2.6%). Subsequently, after 28 days, the strength reduction (µ28%) is 9.8%, 8.7%, 6.9% and 12.2% for mixes with CRCA content of 20%, 40%, 60% and 80%, respectively (µ = 9.9% and σµ = ±2.05%). Moreover, the strength reduction (µ56%) after 56 days is 10.4%, 9.4%, 9.1%, and 18.3% for mixes with CRCA content of 20%, 40%, 60% and 80%, respectively (µ = 11.8% and σµ = ±3.8%). These reductions were due to the CRCA defects that negatively affected their interfacial transition zones (ITZs)). These weak ITZs led to the propagation of the concrete cracks and reduced the strength values [72][73][74][75][76][77]. The lowest values of µ7, µ28 and µ56 are 10.8%, 6.9% and 9.1%, respectively (M3, CRCA = 60%). The mixtures with CRCA (M1-M4) experienced higher differences between µ28/7 and µ56/28 compared to M0 (Table 4). These observations summarize the weak ITZs between the cement paste and CRCA (C-CRCA) besides the CRCA voids. At Tc = 28 days, C-CRCA bond may be enhanced by the hydration of the RCP surrounding CRCA (RCP has a pozzolanic effect as mentioned earlier).
To assess the CRCA effects on the strength gained at 7 and 56 days compared to that at 28 days, the Rc7 (f cu7 /f cu28 ) and Rc56 (f cu56 /f cu28 ) were calculated (Figure 6b) [11,78] that the concrete strength decreased sharply when the coal waste and RCA aggregates replaced NA. Moreover, in [78] a strength reduction of about 26-32% was reported when the RCA aggregates replaced NA. Furthermore, compressive strength reduction of lower than 40% was observed when RAC was incorporated [79]. When the NA was replaced by RCA of 25-50%, the compressive strength reduction was 2-3% depending on the RCA source while when the RCA replacement was more than 50%, the reduction was 15-23% [22]. Based on the above results, basaltic CRCA could be considered as a good substitute for the coarse NA to produce sustainable concrete and reduces the environmental impact and cost of concrete production.

Effect of the RCP
To produce green/sustainable concrete, the RCP was used to partially replace the cement component. The cement was partially substituted by 0%, 5%, 10% and 20% RCP. From Figure 8, the strength increased with increasing Tc value irrespective of the RCP content. When the Tc was increased from 7 to 28 days, the strength increased by 21.20%, 88.81% and 77.39% when the RCP was added with 5%, 10% and 20%, respectively. When the Tc was increased from 28 to 56 days, the strength increased by 6.7%, 3.7% and 11.4% when the RCP was added with 5%, 10% and 20%, respectively. The use of RCP as a replacement material for cement decreased the compressive strength by different percentages depending on the Tc and RCP percentage. After 7 d, the strength decreased by 6.0%, 32.7%, and 36.7% when 5%, 10%, and 20% RCP were added, respectively (µ = 25.12% and σµ = ±13.6%).
The use of RCP as a replacement material for cement decreased the compressive  The effect of FRCA on the strength gained at 7 and 56 days compared to that at 28 days (Rc7% and Rc56%) was calculated (Figure 7b). The figure shows that the Rc7 values were 78.1%, 74.9%, 73.5%, 81.1% and 80.6% when the FRCA was integrated by 0%, 20%, 40%, 60% and 80%, respectively (µ = 77.6% and σ µ = ±3.03%). Moreover, the Rc56 values were 114.7%, 111.8%, 126.0%, 108.8% and 112.4% when the FRCA was added by 0%, 20%, 40%, 60% and 80%, respectively (µ = 114.7% and σ µ = ±5.95%). M6 showed the highest Rc56 value, highlighting the pozzolanic effect of FRCA, which can maintain almost the same M0 strength (99.5%). The incorporation of FRCA into the concrete to replace the natural sand was more efficient than the RA and PA to restore the NAC strength [53]. The previous research studies [35,78] have shown that concrete with RCA has a higher pore structure than concrete with NA. When RCA (coarse and fine) replaced NA, a decrease in strength of about 26-32% was observed in [77] and the same finding was highlighted in [80]. The above observations underlined the suitability of FRCA to produce sustainable concrete with high FRCA replacement ratios.

Effect of the RCP
To produce green/sustainable concrete, the RCP was used to partially replace the cement component. The cement was partially substituted by 0%, 5%, 10% and 20% RCP. From Figure 8, the strength increased with increasing Tc value irrespective of the RCP content. When the Tc was increased from 7 to 28 days, the strength increased by 21.20%, 88.81% and 77.39% when the RCP was added with 5%, 10% and 20%, respectively. When the Tc was increased from 28 to 56 days, the strength increased by 6.7%, 3.7% and 11.4% when the RCP was added with 5%, 10% and 20%, respectively. The use of RCP as a replacement material for cement decreased the compressive strength by different percentages depending on the Tc and RCP percentage. After 7 d, the strength decreased by 6.0%, 32.7%, and 36.7% when 5%, 10%, and 20% RCP were added, respectively (µ = 25.12% and σ µ = ±13.6%).
The use of RCP as a replacement material for cement decreased the compressive strength by different percentages depending on Tc and RCP%. After 7 days, the strength decreased by 6.0%, 32.7% and 36.7% (µ = 25.12% and σ µ = ±13.6%) when 5%, 10% and 20% RCP were added, respectively. Conversely, the strength decreased by 11.0, 0.7 and 12.2% after 28 days when RCP was added by 5%, 10% and 20%, respectively (µ = 7.97% and σ µ = ±5.17%). In addition, the attained strength decreased by 10.4%, 4.80% and 15.2% when RCP was integrated by 5%, 10% and 20%, respectively (µ = 10.13% and σ µ = ±4.95%). The small reduction in strength for mixes with RCP (M9-M11) compared to M0, especially after 28 and 56 days, may be due to the late hydration of RCP. These results assured the pozzolanic effects of RCP, which covered about 99.3% and 95.2% of M0 strength after 28 and 56 days, respectively (RCP = 10%). Moreover, M9 achieved the lowest strength reduction after 7 d (6.0%) with an almost similar difference between µ28/7 and µ56/28 (Table 4). To compare the effect of RCP% on the obtained strength after 7 and 56 d compared to that after 28 d, the Rc7 and Rc56 were calculated (Figure 8b). From the figure, Rc7 was equal to 78.1%, 82.5%, 53% and 56.4% when the RCP was added by 0%, 5%, 10% and 20%, respectively (µ = 67.5% and σ µ = ±12.97%). Moreover, the Rc56 was equal to 114.7%, 115.5%, 110.0% and 110.9% when the RCP was added by 0%, 5%, 10% and 20%, respectively (µ = 112.8% and σ µ = ±2.38%). From all the above, basaltic RCP could be considered as a good substitute for cement to produce green/sustainable concrete, reduce environmental impact and produce concrete with low cost. As reported in [80][81][82], the replacement of cement with SF (5-25%) increases the concrete strength when the recommended superplasticizers are added. The reported and obtained results encourage the use of superplasticizers with the RCP that can regulate their hydration and increase the concrete strength as they have the SF effects on the concrete.

Concrete Tensile Strength
The cubic diagonal tensile strengths (ftu) at ages 28 and 56 days (ftu,28 and ftu,56, respectively) are reported in Table 5 and Figures 9-11. Table 5 shows the increases and decreases in ftu at 28 and 56 days (µt,28 and µt,56, respectively) as a result of the partial replacement of natural basalt, sand, and cement by CRCA, FRCA, and RCP. The percentage increase in ftu,56 compared to ftu,28 (µt56/28) for all tested mixes was also calculated. In addition, the effect of waste concrete components on ftu,28/fcu,28 and ftu,56/fcu,56% was also adopted. The increased/decreased (I/d) percentage in ftu (µt,date%) at each curing time can be calculated using Equation (4).
where ftu,date(R) and ftu,date(N) are the concrete tensile strengths for mixes with recycled components and that with NA, respectively.

Concrete Tensile Strength
The cubic diagonal tensile strengths (f tu ) at ages 28 and 56 days (f tu,28 and f tu,56 , respectively) are reported in Table 5 and Figures 9-11. Table 5 shows the increases and decreases in f tu at 28 and 56 days (µ t, 28 and µ t,56 , respectively) as a result of the partial replacement of natural basalt, sand, and cement by CRCA, FRCA, and RCP. The percentage increase in f tu,56 compared to f tu,28 (µ t56/28 ) for all tested mixes was also calculated. In addition, the effect of waste concrete components on f tu,28 /f cu,28 and f tu,56 /f cu,56 % was also adopted. The increased/decreased (I/d) percentage in f tu (µ t,date %) at each curing time can be calculated using Equation (4).
where f tu,date (R) and f tu,date (N) are the concrete tensile strengths for mixes with recycled components and that with NA, respectively.

Effect of CRCA
Concrete tensile strength was slightly affected by CRCA% and curing time. Increasing the Tc from 28 to 56 days increased the tensile strength at all CRCA% ( Figure 9). The maximum value of increase in ftu was for M3 (CRCA = 60%, µt56/28 = 14.24%). In contrast, the tensile strength decreased with the addition of CRCA compared to mix M0, except for M3 at 56 d (µt56 = 1.98%). The diagonal strength reduced by −3.42%, −2.63%, −1.4% and −2.88% after 28 days, while it reduced by −5.02%, −7.60%, 1.98% and −10.9% after 56 days when CRCA was added by 20%, 40%, 60% and 80%, respectively. M4 (CRCA = 80%) experienced the highest reduction in diagonal strength (µt56 = −10.90%, Table 4). Although the voids in the CRCA negatively affected the tensile strength, the amount of RCP attached to the CRCA could help to reduce the effects of the voids as it produced more gel when hydrated. The comparison of ftu,28/fcu,28% and ftu,56/fcu,56% for the mixtures integrating CRCA with those of M0 ensured the lower effect of CRCA on tensile strength than on compressive strength. The pozzolanic effect of RCP can improve the bond between concrete particles when it contains much basalt powder. In contrast, the CRCA with little basalt powder can interfere with cement hydration by absorbing the hydration water and increasing the voids in the concrete. In addition, the mixes with integrated CRCA had more ITZs than those with NA, which contributed to the detachment of fracture surfaces under tensile loading. In addition, the higher porosity of CRCA concretes resulted in high lateral dilatation compared to concretes with NA, which led to a drastic reduction in compressive strength. The same poor effects of CRCA on compressive strength as on tensile strength were reported in [72,83,84]. Moreover, a tensile strength reduction of about 26-32% was found in [78] when RCA (coarse and fine) was added to replace NA. From the above, the low effect of CRCA makes it a good sustainable replacement material for NA to produce green concrete with low cost and environmental impact with lower tensile strength reduction (µt28 = 3.42% (M1) and µt28 = 10.9% (M4)).

Effect of FRCA
The FRCA was implemented to replace the natural sand in five percentages (0%, 20%, 40%, 60%, and 80%). The concrete diagonal strength was dependent on the FRCA percentage and curing time. Increasing Tc from 28 to 56 d increased the diagonal strength at all FRCA% ( Figure 10) with a maximum enhancement value of 19.78% (M6, FRCA = 40%). Consequently, the diagonal strength of the mixtures with integrated FRCA was higher than that of M0 at 28 and 56 days, except for M5 and M6 at 28 days (Figure 9). After 56 days, diagonal strength increased by 0.26%, 5.40%, 5.40%, and 3.09% when FRCA was added by 20%, 40%, 60%, and 80%, respectively. Moreover, the highest reduction in diagonal strength compared to M0 was equal to −2.88% after 28 days (M6, Table 5). The diagonal strength may depend on the availability of RCP attached to the FRCA. In addition,

Effect of CRCA
Concrete tensile strength was slightly affected by CRCA% and curing time. Increasing the Tc from 28 to 56 days increased the tensile strength at all CRCA% ( Figure 9). The maximum value of increase in f tu was for M3 (CRCA = 60%, µ t56/28 = 14.24%). In contrast, the tensile strength decreased with the addition of CRCA compared to mix M0, except for M3 at 56 d (µ t56 = 1.98%). The diagonal strength reduced by −3.42%, −2.63%, −1.4% and −2.88% after 28 days, while it reduced by −5.02%, −7.60%, 1.98% and −10.9% after 56 days when CRCA was added by 20%, 40%, 60% and 80%, respectively. M4 (CRCA = 80%) experienced the highest reduction in diagonal strength (µ t56 = −10.90%, Table 4). Although the voids in the CRCA negatively affected the tensile strength, the amount of RCP attached to the CRCA could help to reduce the effects of the voids as it produced more gel when hydrated.
The comparison of f tu,28/ f cu,28 % and f tu,56/ f cu,56 % for the mixtures integrating CRCA with those of M0 ensured the lower effect of CRCA on tensile strength than on compressive strength. The pozzolanic effect of RCP can improve the bond between concrete particles when it contains much basalt powder. In contrast, the CRCA with little basalt powder can interfere with cement hydration by absorbing the hydration water and increasing the voids in the concrete. In addition, the mixes with integrated CRCA had more ITZs than those with NA, which contributed to the detachment of fracture surfaces under tensile loading. In addition, the higher porosity of CRCA concretes resulted in high lateral dilatation compared to concretes with NA, which led to a drastic reduction in compressive strength. The same poor effects of CRCA on compressive strength as on tensile strength were reported in [72,83,84]. Moreover, a tensile strength reduction of about 26-32% was found in [78] when RCA (coarse and fine) was added to replace NA. From the above, the low effect of CRCA makes it a good sustainable replacement material for NA to produce green concrete with low cost and environmental impact with lower tensile strength reduction (µ t28 = 3.42% (M1) and µ t28 = 10.9% (M4)).

Effect of FRCA
The FRCA was implemented to replace the natural sand in five percentages (0%, 20%, 40%, 60%, and 80%). The concrete diagonal strength was dependent on the FRCA percentage and curing time. Increasing Tc from 28 to 56 d increased the diagonal strength at all FRCA% ( Figure 10) with a maximum enhancement value of 19.78% (M6, FRCA = 40%). Consequently, the diagonal strength of the mixtures with integrated FRCA was higher than that of M0 at 28 and 56 days, except for M5 and M6 at 28 days (Figure 9). After 56 days, diagonal strength increased by 0.26%, 5.40%, 5.40%, and 3.09% when FRCA was added by 20%, 40%, 60%, and 80%, respectively. Moreover, the highest reduction in diagonal strength compared to M0 was equal to −2.88% after 28 days (M6, Table 5). The diagonal strength may depend on the availability of RCP attached to the FRCA. In addition, the fine basalt aggregates may act as microfibers that help to suppress the internal macrocracks and increase the diagonal strength values.
Comparing the f tu,28/ f cu,28 % and f tu,56/ f cu,56 % for the mixes containing the FRCA with those of M0, the significant effect of the FRCA on the diagonal strength was greater than that on the compressive strength. The pozzolanic effect of RCP can improve the bond between concrete particles. The failure of the cubes followed the diagonal failure characteristics (Figure 11), as reported in [67]. Finally, the FRCA trivially diminished the f cu values while amplified the f tu values. The previous results and comparisons encouraged the use of recycled aggregates as a substitute material for the NA to produce green concrete.
In contrast to the effect of RA and PA, the incorporation of FRCA into concrete increased f tu values compared to NAC [53].

Effect of the RCP
To emphasize the pozzolanic effect of RCP on concrete properties, the tensile strength of mixes integrating RCP was tested ( Figure 12). From Figure 12, the diagonal strength for the mixes integrating RCP increased with increasing curing time regardless of the RCP content. When Tc was increased from 28 to 56 days, the diagonal strength increased by 6.68%, 3.72% and 11.44% when RCP was added by 5%, 10% and 20%, respectively. This could be due to the hydration of the remaining un-hydrated cement and the late hydration of the basalt fines and powder. Consequently, replacing the cement with 5% and 10% RCP increased the 28 days tensile strength by 6.81% and 6.81%, respectively, while the 56 days tensile strength increased by 3.09 and 0.26%, respectively, compared to M0. In contrast, for mixes integrating 20% RCP, the tensile strength at 28 and 56 days decreased by −2.92% and −2.05%, respectively, compared to that of M0. Conversely, the f tu,28/ f cu,28 % and f tu,56/ f cu,56 % increased with the incorporation of RCP compared to M0. The pozzolanic effect of RCP may enhance the bond between concrete particles. The results are in agreement with those in [35] which stated that the effect of RCA can be controlled by careful selection during concrete production. In fact, the loss or increase of tensile strength was dependent on the type, size, quantity, and quality of RCA. the fine basalt aggregates may act as microfibers that help to suppress the internal macrocracks and increase the diagonal strength values. Comparing the ftu,28/fcu,28% and ftu,56/fcu,56% for the mixes containing the FRCA with those of M0, the significant effect of the FRCA on the diagonal strength was greater than that on the compressive strength. The pozzolanic effect of RCP can improve the bond between concrete particles. The failure of the cubes followed the diagonal failure characteristics (Figure 11), as reported in [67]. Finally, the FRCA trivially diminished the fcu values while amplified the ftu values. The previous results and comparisons encouraged the use of recycled aggregates as a substitute material for the NA to produce green concrete.
In contrast to the effect of RA and PA, the incorporation of FRCA into concrete increased ftu values compared to NAC [53].

Effect of the RCP
To emphasize the pozzolanic effect of RCP on concrete properties, the tensile strength of mixes integrating RCP was tested ( Figure 12). From Figure 12, the diagonal strength for the mixes integrating RCP increased with increasing curing time regardless of the RCP content. When Tc was increased from 28 to 56 days, the diagonal strength increased by 6.68%, 3.72% and 11.44% when RCP was added by 5%, 10% and 20%, respectively. This could be due to the hydration of the remaining un-hydrated cement and the late hydration of the basalt fines and powder. Consequently, replacing the cement with 5% and 10% RCP increased the 28 days tensile strength by 6.81% and 6.81%, respectively, while the 56 days tensile strength increased by 3.09 and 0.26%, respectively, compared to M0. In contrast, for mixes integrating 20% RCP, the tensile strength at 28 and 56 days decreased by −2.92% and −2.05%, respectively, compared to that of M0. Conversely, the ftu,28/fcu,28% and ftu,56/fcu,56% increased with the incorporation of RCP compared to M0. The pozzolanic effect of RCP may enhance the bond between concrete particles. The results are in agreement with those in [35] which stated that the effect of RCA can be controlled by careful selection during concrete production. In fact, the loss or increase of tensile strength was dependent on the type, size, quantity, and quality of RCA.

Water Absorption
To examine the effect of CRCA, FRCA and RCP on concrete durability, the water absorption (WA) was calculated for all concrete mixes after 28 and 56 days (Figure 13). In general, all mixes had lower WA values after 56 days than their WA values after 28 days, except for mixes M2, M7, and M8 ( Figure 13). This is because of the excessive hydration of the cement, which increased the C-S-H gel and decreased the voids. In addition, the

Water Absorption
To examine the effect of CRCA, FRCA and RCP on concrete durability, the water absorption (WA) was calculated for all concrete mixes after 28 and 56 days (Figure 13). In general, all mixes had lower WA values after 56 days than their WA values after 28 days, except for mixes M2, M7, and M8 ( Figure 13). This is because of the excessive hydration of the cement, which increased the C-S-H gel and decreased the voids. In addition, the WA values at the same Tc were dependent on the type and percentages of recycled materials. The WA of mixtures M1-M4 (with integrated CRCA) increased with increasing CRCA content at 28 d (Figure 13a). Similar effects of CRCA content on WA values were observed after 56 days for the same mixtures except for M2. The WA of mixtures M1-M4 was higher than that of mixture M0 (Figure 13a). This may be due to the high void content of CRCA as it involves crushed mortar. The previous observations were previously reported in [85][86][87]. Similarly, at 28 and 56 d, mixtures M5-M8 had higher WA values than those of M0 (Figure 13b). Among the mixtures integrating FRCA, both mixtures M6 (FRCA = 40%) and M7 (FRCA = 60%) experienced the lowest WA values at 56 and 28 days, respectively. The WA of the mixes with FRCA may depend on the amount of crushed concrete and the hydration of the fines incorporated in the FRCA. Conversely, cement preplacement with 5% and 10% RCP had a small effect on WA values at 28 and 56 d, while increasing RCP to 20% increased WA (Figure 13c). When RCP replaced cement up to 10%, the effect of RCP on cement hydration was negligible and RCP could store almost the same C-S-H gel as cement, while increasing RCP to 20% may disturb cement hydration and affect the production of C-S-H gel in the mix.
WA values at the same Tc were dependent on the type and percentages of recycled materials. The WA of mixtures M1-M4 (with integrated CRCA) increased with increasing CRCA content at 28 d (Figure 13a). Similar effects of CRCA content on WA values were observed after 56 days for the same mixtures except for M2. The WA of mixtures M1-M4 was higher than that of mixture M0 (Figure 13a). This may be due to the high void content of CRCA as it involves crushed mortar. The previous observations were previously reported in [85][86][87]. Similarly, at 28 and 56 d, mixtures M5-M8 had higher WA values than those of M0 (Figure 13b). Among the mixtures integrating FRCA, both mixtures M6 (FRCA = 40%) and M7 (FRCA = 60%) experienced the lowest WA values at 56 and 28 days, respectively. The WA of the mixes with FRCA may depend on the amount of crushed concrete and the hydration of the fines incorporated in the FRCA. Conversely, cement preplacement with 5% and 10% RCP had a small effect on WA values at 28 and 56 d, while increasing RCP to 20% increased WA (Figure 13c). When RCP replaced cement up to 10%, the effect of RCP on cement hydration was negligible and RCP could store almost the same C-S-H gel as cement, while increasing RCP to 20% may disturb cement hydration and affect the production of C-S-H gel in the mix.

Theoretical and Experimental Comparisons
The proposed model reported in [62] was used to predict the RAC compressive and tensile strength. The relationship between the theoretical findings and the obtained experimental results is shown in Figure 14. The theoretical compressive and tensile strength were evaluated using Equations (5) and (6), respectively as follows.

Theoretical and Experimental Comparisons
The proposed model reported in [62] was used to predict the RAC compressive and tensile strength. The relationship between the theoretical findings and the obtained experimental results is shown in Figure 14. The theoretical compressive and tensile strength were evaluated using Equations (5) and (6) (6) The model can predict with good accuracy the compressive and tensile strength of the RAC as shown in Figure 14.
The model can predict with good accuracy the compressive and tensile strength of the RAC as shown in Figure 14.

Conclusions
The strength and durability of green concrete produced with recycled basaltic concrete aggregates and powder were investigated. The effect of RCA, FRNA and RCP as substitutes for the concrete constituents (NA and cement) on the strength and durability of concrete was evaluated experimentally at different test ages. The conclusions obtained are given as follows: • With increasing curing time, concrete compressive and tensile strengths increased regardless of the concrete components (with or without recycled materials). The concrete strength increased with increasing Tc from 7 to 28 days with a higher percentage than increasing Tc from 28 to 56 days. This may be because of the higher hydration rate of the cement during the first 28 days compared to the later days. • Partial substitution of recycled aggregate for NA reduced concrete strength with varying percentages depending on the size and source of recycled aggregate, especially after 56 days. After 28 days, the maximum reduction in concrete strength when CRCA or FRCA was incorporated up to 80% was 7.6% and 4.6%, respectively, while the maximum reduction in strength was 13

Conclusions
The strength and durability of green concrete produced with recycled basaltic concrete aggregates and powder were investigated. The effect of RCA, FRNA and RCP as substitutes for the concrete constituents (NA and cement) on the strength and durability of concrete was evaluated experimentally at different test ages. The conclusions obtained are given as follows: • With increasing curing time, concrete compressive and tensile strengths increased regardless of the concrete components (with or without recycled materials). The concrete strength increased with increasing Tc from 7 to 28 days with a higher percentage than increasing Tc from 28 to 56 days. This may be because of the higher hydration rate of the cement during the first 28 days compared to the later days. • Partial substitution of recycled aggregate for NA reduced concrete strength with varying percentages depending on the size and source of recycled aggregate, especially after 56 days. After 28 days, the maximum reduction in concrete strength when CRCA or FRCA was incorporated up to 80% was 7.6% and 4.6%, respectively, while the maximum reduction in strength was 13 The obtained results and comparisons encourage the use of recycled aggregates and powders as a substitute material for NA and cement to produce sustainable/green concrete.

•
The recycled aggregates could obtain nearly the same mechanical properties of mixes with natural aggregate. Conversely, the use of RCP to replace cement also reduces the cost and CO 2 emission from the cement production process. So, the use of recycled aggregates and powder to replace the natural aggregate and cement, respectively could be considered an efficient method to lower the structures' cost, their impact on the environment, and improves their sustainability.

•
The transportation costs of natural aggregate and other construction materials have significant effects on the economic analysis. The use of recycled aggregate in rebuilding, demolition and retrofitting of structures could be very effective as the source of the old concrete is near to the construction site.